\begin{figure}
\beginpicture
\setcoordinatesystem units <1mm,1mm>
\put {~} at -27 0
\tickstovaluesleading10pt
\longticklength4pt
\shortticklength2pt
\setplotarea x from 0 to 90, y from 0 to 60

\axis bottom
        label {$t / \mathrm{min}$}
        ticks in withvalues 0 30 60 90 120 /
        quantity 5 short quantity 9
        /
\axis left
        label {$c / \mathrm{M}$}
        ticks in withvalues 0 0.3 0.6 0.9 1.2 /
        quantity 5 short quantity 9
        /
\axis top
        ticks in quantity 5 short quantity 9
        /
\axis right
        ticks in quantity 5 short quantity 9
        /

\inboundscheckon
\setquadratic

\plot
0	52
4.3030	51.5835
4.8771	51.4800
5.5287	51.3465
5.8868	51.2665
6.2684	51.1755
6.6752	51.0725
7.1087	50.9560
7.5709	50.8235
8.0637	50.6740
8.5892	50.5040
9.1499	50.3120
9.7480	50.0940
10.3863	49.8467
11.0678	49.5665
11.7954	49.2488
12.5728	48.8885
13.4036	48.4799
14.2919	48.0163
15.2424	47.4902
16.2599	46.8931
17.3501	46.2151
18.5192	45.4448
19.7743	44.5695
21.1234	43.5741
22.5758	42.4413
24.1425	41.1510
25.8364	39.6797
27.6735	37.9995
29.6737	36.0773
31.8629	33.8726
34.2765	31.3354
36.9648	28.4015
40.0049	24.9866
43.5214	20.9784
47.7058	16.2674
52.5377	11.1776
56.6996	7.3845
59.7641	5.0911
62.3981	3.5111
64.5914	2.4784
66.5091	1.7750
68.2152	1.2899
69.7682	0.9482
71.2056	0.7036
72.5552	0.5260
73.8368	0.3955
75.0653	0.2988
76.2510	0.2265
77.4023	0.1722
78.5258	0.1311
79.6260	0.1000
80.7068	0.0764
81.2408	0.0667
82.2975	0.0510
/

\multiput {$\diamond$} at
0.000	52.000
13.500	48.464
18.750	45.188
23.250	40.768
27.000	36.660
32.250	30.732
36.750	24.804
43.500	16.536
49.500	12.428
56.250	6.500
60.000	4.160
63.750	2.340
67.500	0.676
71.250	0.000
/

\multiput {$\circ$} at
0.000	52.000
7.500	50.024
15.000	47.216
22.500	41.236
30.000	33.644
37.500	25.428
45.000	18.096
52.500	11.284
60.000	5.668
63.750	2.288
67.500	1.144
71.250	0.000
/

\multiput {\tiny$\Box$} at
0.000	52.000
7.500	51.376
15.000	48.880
22.500	44.252
30.000	37.440
38.250	28.496
45.750	20.748
54.000	13.624
60.000	9.308
63.750	6.812
67.500	4.316
71.250	2.496
75.000	1.248
78.750	0.000
/

\endpicture

\caption{
Vergleich der experimentell bestimmten Abhängigkeit der 
{\footnotesize MMA}-Konzentration von der Zeit
für die Polymerisation von {\footnotesize MMA} mit {\bf 1} und {\bf 6}
mit den theoretischen Funktionen. 
Reaktionsbedingungen: siehe Abbildung 3.1,
$[{\bf 6}]_0 = \unit[1.00]{mM}$.\newline
$\diamond 		: [{\bf 1}]_0 = \unit[6.00]{mM}$,
$\circ 	: [{\bf 1}]_0 = \unit[4.00]{mM}$,
{\tiny$\Box$}
$: [{\bf 1}]_0 = \unit[2.00]{mM}$.
}

\end{figure}
